Luis Fernando Barral Losada y Rebeca Bouza Padín, como directores de la Tesis Doctoral de Yousof Ramadan Farrag AbdEl Hafez, con NIE nº Y2216064M, autorizamos su presentación para depósito.
Synthesis and characterization of nano
and microparticles of biopolymers for
food packaging applications.
Author: Yousof Farrag
Doctoral Thesis UDC / 2017
Directors: Dr. Rebeca Bouza Padín
Dr. Luis Fernando Barral Losada
Doctoral program of Applied Physics
It is only my name will be written as the author of this work, but in fact many people deserve to have their names there, even before mine.
I would like to start thanking my parents. You have been by my side during all my entire life and especially during the master and the PhD research. You believed in me, supported and encouraged me with all that you could. Without you, all this work would not have been possible. No words would be sufficient to thank you. I love you so much. Thanks a lot, from all my heart.
I would like to express my gratitude to my supervisors: prof. Luis Barral and prof. Rebeca Bouza. Thank you for your confidence in me, supporting me, being patients with me, for all what I have learned from you and for motivating me especially in the difficult moments. Luis, you taught me a lot, at the scientific level and in general life aspects. I am eternally grateful to you for your continuous help and support. At the same time, you did encourage me to try and develop my own ideas. Thank you.
also for translating the spanish parts of this thesis.
To my sisters Omima and Mariam, many thanks to you for your support. I am lucky to have you in my life.
I would like to acknowledge the help and support I received from the people of the (Centro de Investigación de Polímeros Avanzados, CIPA, Chile). Dr. Saddys Rodríguez-Llamazares, thank you for the time, the effort and the contributions to this work. To Walther Ide, Constanza Sabando and Natalia Pettinelli, thank you for your collaboration and for the effort you put into this work.
To prof. Tomas Torres, you opened to me the door to the investigation here in Spain. It is an honour to be your student. I am grateful for all what you have done for me.
To my friend Hytham Ahmad, it is really hard to find a sincere person like you in these days. You guided me to my first steps to the scientific research. Thank you.
have learned a lot from our discussions. It was an honour working with you.
I would like to thank all the members of the group of polymers especially Sara, Belén, Maite, Jesús, María del Carmen, Javier and Joaquin. Thank you all for your support. My special thanks to the lab technician, Ángeles, for your effort and precise work.
I would not forget my friends and colleagues from the Complutense University of Madrid: Paulino, Marco, David, Diego, Ana and Monte. I spent an amazing time with you. I have learned a lot from all of you. Thank you.
Many thanks to everyone who helped me during this work. Belen Cuesta from CiMUS; Raquel Antón, the FESEM technician; Dr. Alberto Nuñez from the structural analysis unit of SAI, thank you all for your contributions.
Thanks to everyone who taught me even a letter in my life, to all my friends, teachers and all my family.
The main aim of this thesis is the preparation and characterization of nano and microparticles of selected biopolymers addressed for food packaging and active food packaging applications.
Two biopolymers have been selected for the nano and microparticles preparations: poly(3-hydroxybutyrate-co-3-hydroxyvalerate) (PHBV) and starch. The results for the PHBV showed spherical porous particles with wide variety of size distribution depending on the selected techniques and the procedure conditions. Starches from different botanical origins were used for preparing starch nanoparticles and starch/quercetin nanoparticles using the nanoprecipitation technique. The loading capacity, the release profile of the quercetin from the nanoparticles and therefore the antioxidant activity changed by changing the starch origin.
kept releasing during 4 to 11 days depending on the starch origin. The produced nano and microparticles provide many
possibilities for improving some properties of the biopolymeric
packaging films with the capacity for active delivery function for
El objetivo de esta tesis es la preparación y caracterización de nano y micropartículas de biopolímeros para su uso en envases y embalajes alimentarios convencionales y activos.
Se seleccionaron dos biopolímeros: Poli(3-hidroxibutirato-co-3-hidroxivalerato) (PHBV) y almidón. Para el PHBV, los resultados mostraron partículas esféricas y porosas con una amplia variedad en la distribución de tamaños, en función de la técnica utilizada y las condiciones de preparación. Se han utilizado también almidones de diferentes orígenes botánicos en la preparación de las nanopartículas tanto de almidón solo como de almidón cargado con quercetina. La capacidad de carga, el perfil de liberación y el consiguiente cambio en la actividad antioxidante de la quercetina varía según el origen del almidón.
O obxectivo desta tese é a preparación e caracterización de nano e micropartículas de biopolímeros para o seu uso en envases e embalaxes alimentarios convencionais e activos.
Seleccionáronse dous biopolímeros: Poli(3-hidroxibutirato-co-3-hidroxivalerato (PHBV) e amidón. No caso do PHBV, os resultados amosaron partículas esféricas e porosas cunha ampla variedade na distribución de tamaños en función da técnica utilizada e as condicións de preparación.
Tamén, utilizáronse amidóns de orixes botánicas diferentes na preparación das nanopartículas, tanto as de só amidón como as de amidón cargado con quercetina. A capacidade de carga, o perfil de liberación e o cambio na actividade antioxidante da quercetina varía segundo a orixe do amidón.
Abstract ... 1 2. Bioplastics and biopolymers ... 31 2.1. Polyhydroxyalkanoates (PHAs) ... 33 2.2. Polysaccharides ... 34 3. Biopolymers for food packaging ... 36 4. Materials and characterization techniques ... 44 4.1. Materials ... 44 4.1.1. Poly(3-hydroxybutyrate-co-3-hydroxyvalerate) ... 44 4.1.2. Starch ... 46 4.1.3. Quercetin ... 50 4.2. Characterization techniques ... 52 4.2.1. Scanning electron microscopy (SEM) ... 52 4.2.2. Dynamic light scattering (DLS) ... 54 4.2.3. Static light scattering (SLS) ... 56 4.2.4. Thermogravimetric analysis (TGA) ... 56 4.2.5. Differential scanning calorimetry (DSC) ... 57 4.2.6. X-ray diffraction (XRD) ... 59 4.2.7. Ultraviolet–visible spectroscopy (UV–vis) ... 60 4.2.8. Water vapour transmission rate (WVTR) ... 62 4.2.9. Oxygen transmission rate (OTR) ... 63 Objectives of the Thesis ... 66 Structure of the Thesis ... 67 References ... 72
techniques ... 80
1. Introduction ... 81 2. Materials and methods ... 86 2.1. Materials and reagents ... 86 2.2. Preparation of the particles via emulsification/solvent
evaporation ... 86 2.3. Preparation of the particles via nanoprecipitation ... 89 2.4. Characterization ... 92 3. Results and discussion. ... 92 3.1. Emulsification/solvent evaporation ... 92 3.1.1. Emulsification using SDS ... 93 3.1.2. Emulsification using PVA ... 100 3.2. Nanoprecipitation ... 107 3.2.1. Ethanol as anti-solvent ... 107 3.2.2. Methanol as anti-solvent ... 110 3.2.3. Water as anti-solvent ... 114 4. Conclusions ... 115 References ... 118
3. Preparation of starch nanoparticles loaded with quercetin using nanoprecipitation technique. ... 127
4. Preparation of donut-shaped starch microparticles by
aqueous-alcoholic treatment ... 168
1. Introduction ... 169 2. Materials and methods ... 171 2.1. Materials and reagents ... 171 2.2. Preparation of starch microparticles ... 171 2.3. Scanning electron microscopy (SEM) ... 172 2.4. X-ray diffraction (XRD) ... 172 2.5. Differential scanning calorimetry (DSC) ... 173 2.6. Solubility and swelling properties ... 173 3. Results and discussion ... 175 3.1. Scanning electron microscopy (SEM) ... 175 3.2. X-ray diffraction (XRD) ... 177 3.3. Differential scanning calorimetry (DSC) ... 179 3.4. Solubility and swelling properties ... 182 4. Conclusions ... 184 References ... 186
5. Starch edible films loaded with donut-shaped starch
microparticles ... 189
1. Introduction ... 190 2. Materials and methods ... 192 2.1. Materials and reagents ... 192 2.2. Preparation of starch microparticles. ... 192 2.3. Preparation of starch films loaded with donut-shaped starch microparticles ... 193 2.4. Scanning electron microscopy (SEM) ... 194 2.5. Solubility and swelling properties ... 195 2.6. X-ray diffraction (XRD) ... 196 2.7. Thermogravimetric analysis (TGA) ... 196 2.8. Water vapour transmission rate (WVTR) ... 197 2.9. Oxygen transmission rate (OTR) ... 197 3. Results and discussion ... 199
3.1. Preparation and characterization of the donut-shaped starch microparticles ... 199
loaded TPS ... 206 3.2.1. Morphology ... 206 3.2.2. X-ray diffraction analysis (XRD) ... 207 3.2.3. Thermogravimetric analysis (TGA) ... 210 3.2.4. Water vapour and oxygen transmission rates ... 212 4. Conclusions ... 213 References ... 215
6. Starch edible films loaded with donut-shaped
starch-quercetin microparticles: characterization and release kinetics ... 219
1. Introduction ... 220 2. Materials and methods ... 222 2.1. Materials and reagents ... 222 2.2. Preparation of starch-quercetin microparticles. ... 223 2.3. Preparation of starch films loaded with donut-shaped starch-quercetin microparticles ... 224 2.4. Scanning electron microscopy (SEM) ... 225 2.5. Determination of quercetin loading percentage ... 225 2.6. Antioxidant activity ... 226 2.7. Thermogravimetric analysis (TGA) ... 228 2.8. In-vitro release in water/ethanol medium ... 228 2.9. Statistical analysis ... 229 3. Results and discussion ... 229
3.1. Preparation and characterization of the starch-quercetin
microparticles ... 229 3.2. Loading percentage and antioxidant activity ... 232 3.3. Thermogravimetric analysis (TGA) ... 235 3.4. Quercetin release kinetics from the starch films ... 237 4. Conclusions ... 245 References ... 247
7. General conclusions ... 252 Anexo I: Resumen ... 256
Figure 1.1 Plastic types as a function of natural sources and
biodegradability (European bioplastics, 2017b). ... 31 Figure 1.2 General chemical structure of PHAs ... 34 Figure 1.3 Glycosidic bonds in an amylopectin molecule. ... 35 Figure 1.4 Global production capacities of bioplastics by market
segment (European bioplastics, 2016). ... 37 Figure 1.5 Schematic representation of the chemical structure of
PHBV ... 45 Figure 1.6 Schematic representation of amylose. ... 49 Figure 1.7 Schematic representation of amylopectin. ... 49 Figure 1.8 Skeletal formula of quercetin. ... 51 Figure 1.9 Diagram of FESEM. ... 53 Figure 1.10 Diagram of bragg's diffraction. ... 60 Figure 1.11 Diagram of a WVTR testing cell. ... 63 Figure 1.12 Diagram of an OTR testing cell. ... 64 Figure 2.13 Micrograph of a microparticle of PHBV prepared by
emulsification/solvent evaporation method using 1% PHBV in dichloromethane and SDS as surfactant in a concentration of 1% (2ES). ... 93 Figure 2.14 Static light scattering plot. Particle diameter in µm vs
prepared by emulsification/solvent evaporation method using 1% PHBV in dichloromethane and SDS as surfactant with concentrations: 0.3% (a: 1ES), 1% (b: 2ES), 2% (c: 3ES), 5% (d: 4ES), 10% (e: 5ES), 15% (f: 6ES). ... 96 Figure 2.16 Micrograph of nano and microparticles of PHBV
prepared by emulsification/solvent evaporation method using SDS as surfactant with concentrations: 1% PHBV, 1% SDS (a: 2ES), 0.1% PHBV 1% SDS (b: 7ES), 1% PHBV 2% SDS (c: 3ES), 0.1% PHBV 2% SDS (d: 8ES), 1% PHBV 5% SDS (e: 4ES), 0.1% PHBV 5% SDS (f: 9ES), 1% PHBV 10% SDS (g: 5ES), 0.1% PHBV 10% SDS (h: 10ES). ... 98 Figure 2.17 Static light scattering plot. Particle diameter in µm vs
incremental volume percent for different PHBV samples prepared by emulsification/solvent evaporation using different concentrations of SDS as surfactant and polymer
concentration of 0.1%. ... 99 Figure 2.18 Static light scattering plot. Particle diameter in µm vs
incremental volume percent for different PHBV samples prepared by emulsification/solvent evaporation using different concentrations of PVA as surfactant and polymer
concentration of 1%. ... 101 Figure 2.19 Micrograph of nano and microparticles of PHBV
prepared by emulsification/solvent evaporation method using PVA as surfactant with concentrations: 1% PHBV 4% / PVA (a: 12ES), 1% PHBV / 5%PVA (b: 13ES), 1% PHBV / 10% PVA (c: 14ES), 0.5% PHBV 10% PVA (d: 15ES). ... 101 Figure 2.20 Static mode light scattering plot. Particle diameter in
µm vs incremental volume percent for different PHBV
samples prepared by emulsification/solvent evaporation using solution of 10% PVA as surfactant and three different
polymer concentrations. ... 103 Figure 2.21 Dynamic light scattering plot showing the size
dichloromethane using two different surfactants, SDS (11ES) and PVA (17ES) applying the ultrasonication instead of stirring for emulsion preparation. ... 106 Figure 2.22 Micrograph of nano and microparticles of PHBV
prepared by nanoprecipitation method using 1% PHBV in dichloromethane and a mixture of ethanol and water as anti-solvent: 100% ethanol (a: 1NE), 80% ethanol/20% water (b: 7NE), 70% ethanol/30% water (c: 8NE), 70% ethanol/30% water applying ultrasonication (d: 9NE). ... 108 Figure 2.23 Dynamic light scattering plot showing the size
distribution of PHBV nanoparticles prepared by
nanoprecipitation of 1% PHBV in dichloromethane using 70% ethanol/30% water applying ultrasonication (9NE). ... 109 Figure 2.24 Micrograph of nano and microparticles of PHBV
prepared by nanoprecipitation method using: 0.1% PHBV / 90% methanol + 10% water (a: 13NM), 0.1% PHBV / 80% methanol+20% water (b: 16NM), 0.1% PHBV / 70%
methanol+30% water (c: 19NM), 1% PHBV / 90% methanol + 10% water (d: 14NM), 1% PHBV /80% methanol+20% water (e: 17NM), 1% PHBV / 70% methanol+30% water (f: 20NM). ... 111 Figure 2.25 Dynamic light scattering plot showing the size
distribution of PHBV particles prepared by nanoprecipitation of 0.1% PHBV in dichloromethane using different mixtures of methanol and water as anti-solvents. ... 113 Figure 2.26 Micrograph of nano and microparticles of PHBV
prepared by nanoprecipitation method using 0.5% PHBV in DMF as solvent and water as anti-solvent (a: 22NW), 0.1% PHBV in DMF as solvent and 10% NaCl solution in water as anti-solvent (b: 24NW). ... 114 Figure 3.27 Micrograph of pea (a), potato (b) and corn (c) starch
quercetin nanoparticles. ... 144 Figure 3.29 Cumulative release profiles of quercetin from
starch-quercetin nanoparticles from different origins. ... 148 Figure 3.30 Radical scavenging activity (%) for different volumes
of the starch-quercetin nanoparticles suspensions and for the row quercetin solution as positive control. ... 149 Figure 3.31 Fit of various mathematical models to the experimental
release data of the quercetin from the potato starch
nanoparticles. ... 153 Figure 3.32 Fit of the Peppas-Sahlin model to the experimental
release data of quercetin from nanoparticles of starches from different botanical origin. ... 155 Figure 4.33: Representative SEM images (A, C, D) and size
distribution of outer and inner diameter (B) of donut-shaped microparticles. ... 175 Figure 4.34: XRD diffraction patterns of corn starch granules and
donut-shaped microparticles. ... 179 Figure 4.35: DSC curves of corn starch granules and donut-shaped
microparticles. ... 181 Figure 5.36 SEM micrographs of donut-shaped microparticles of
corn (a, b) and pea (c, d) starch. ... 199 Figure 5.37 XRD diffraction patterns of starch granules and their
donut-shaped microparticles of corn (a) and pea (b). ... 202 Figure 5.38 SEM micrographs of the TPS surfaces: a) corn starch,
b) corn starch + 10% microparticles, c) corn starch + 15% microparticles, d) pea starch, e) pea starch + 10%
microparticles, f) pea starch + 15% microparticles. ... 206 Figure 5.39. XRD diffraction patterns of starch granules and their
(b). ... 211 Figure 6.41 SEM micrographs of the starch-quercetin donut shaped
microparticles of corn (a) and pea (b) starches. ... 230 Figure 6.42 Antioxidant activity of the starch-quercetin
microparticles and quercetin standard solutions. ... 233 Figure 6.43 TGA and DTG curves of the starch-quercetin
microparticles and the starch granules (a) and of the starch films containing starch-quercetin microparticles (b). ... 235 Figure 6.44 Release kinetics of quercetin from starch films loaded
with starch-quercetin microparticles of the same botanical origin (corn (a) and pea (b)). ... 238 Figure 6.45 Absorbance graphs of the pea starch film containing
15% pea starch-quercetin microparticles at 6 h and 264 h. The absorbance at 264 h was recorded after dilution. ... 239 Figure 6.46 Fit of the Peppas-Sahlin model to the experimental
Table 1.1 Common plastics and their major applications
(Encyclopædia Britannica, 2017). ... 28 Table 1.2 Classification and examples of bio-based plastics
according to their origin ... 32 Table 1.3 Thermal and mechanical properties of some common bio and conventional plastics in food packaging Sources: (Avella, Martuscelli, & Raimo, 2000; Encyclopædia Britannica, 2017; Stevens, 2003). ... 39 Table 1.4 Melting temperatures and degree of crystallinity of PHB
and different types of PHBV. ... 46 Table 2.5 Preparation conditions of PHBV particles via
emulsification/solvent evaporation. ... 88 Table 2.6 Preparation conditions of PHBV particles via
nanoprecipitation. ... 91 Table 3.7 Dynamic light scattering data for different starch
nanoparticles samples. ... 142 Table 3.8 Parameters obtained by fitting the quercetin release
profiles to different release models. ... 152 Table 4.9 Thermal properties, swelling power and solubility of
corn starch and donut microparticles. ... 181 Table 5.10 Particle size analysis and solubility properties of the
starch granules and their corresponding donut-shaped
microparticles ... 201 Table 5.11 Water vapour permeability and Oxygen permeability
values for starch films ... 212 Table 6.12 Parameters obtained by fitting the quercetin release
ABS Acrylonitrile-butadiene-styrene CNC Cellulose nanocrystals
DLS Dynamic light scattering DNA Deoxyribonucleic acid
DSC Differential scanning calorimetry
FESEM Field emission scanning electron microscopes
GHG Greenhouse gases
HDPE High-density polyethylene (HDPE)
LDPE Low-density polyethylene OTR Oxygen transmission rate PBS Polybutylene succinate PCL Polycaprolactone
PET Polyethylene terephthalate PHAs Polyhydroxyalkanoates
PVD Physical vapour deposition RNA Ribonucleic acid
SLS Static light scattering TGA Thermogravimetric analysis TPS Thermoplastic starch
Table 1.1 Common plastics and their major applications (Encyclopædia Britannica, 2017).
Polymer family and type Typical products and applications High-density polyethylene
Milk bottles, wire and cable insulation, toys
(LDPE) Packaging film, grocery bags, agricultural mulch Polypropylene (PP) Bottles, food containers, toys Polystyrene (PS) Eating utensils, foamed food
(PET) Transparent bottles, recording tape Polyester (unsaturated)
(PES) Boat hulls, automobile panels
Polyurethane (PUR) Flexible and rigid foams for upholstery, insulation
2. Bioplastics and biopolymers
Figure 1.1 Plastic types as a function of natural sources and biodegradability (European bioplastics, 2017b).
Those bio-based and biodegradable polymers that are produced naturally by living organisms are considered biopolymers. Table 1.2 resumes the classification and some examples of the bio-based plastics according to their origin.
Table 1.2 Classification and examples of bio-based plastics according to their origin
2.1. Polyhydroxyalkanoates (PHAs)
PHAs are linear polyesters that are produced by some microorganisms to store carbon and energy for metabolizing them in absence of external carbon source. These polymers are accumulated in the cytoplasm of the cell forming up to 95% of the dry cell weight. The biopolymers can be extracted with a solvent then precipitated from water as a white powder (Stevens, 2003). Some PHAs are produced commercially by large scale fermentation in bioreactors.
Figure 1.2 General chemical structure of PHAs
PHAs are biocompatible biopolymers and some of them have biomedical applications. The biocompatibility of a material deals with how the tissue reacts to foreign materials and the ability of a material to perform with an appropriate host response in a specific application (Kumar et al., 2003). They are also completely biodegradable biopolymers where the biodegradation depends on copolymer composition, molecular weight, degree of crystallinity and the size and shape of the article (Stevens, 2003).
(Daintith, 2008). Monosaccharides units are connected through glycosidic bonds [Figure 1.3].
Figure 1.3 Glycosidic bonds in an amylopectin molecule.
the rigidity of the cell wall of many plants, algae and some fungi. It also has wide industrial applications as paper, textile, food and pharmaceutical industries. Starch is one of the most important polysaccharides for many industries and represents energy source for the humans as the most common carbohydrate in human diets. More detailed information about starch will be given later in this chapter.
3. Biopolymers for food packaging
Although the market of bioplastics is still young and shares only around 1% of the global plastic market, the demand on the bioplastics is rising and new bioplastic products are developed continuously every year. The growth of the bioplastic market is reaching between 20% and 100% per year (European bioplastics, 2016). The production of some bioplastics like the polyhydroxyalkanoates PHAs is expected to quadruple by 2021. As in the case of conventional plastics, packaging is the largest field of applications for the bioplastics with around 39% of the total bioplastic markets in 2016 [Figure 1.4].
Table 1.3 Thermal and mechanical properties of some common bio and conventional plastics in food packaging Sources: (Avella, Martuscelli, &
Raimo, 2000; Encyclopædia Britannica, 2017; Stevens, 2003).
deformability (Imre & Pukánszky, 2013). The use of plasticizers improves the mechanical properties and decrease the glass transitions and the melting points of polymers improving their processability (Mousa, Dong, & Davies, 2016). Physical blending is the simple mixing of polymers during melt state when no chemical reaction is taking place. Several studies were published reporting blends of several biopolymers including blending of starch with PLA, PHB, PCL; PHB with PHBV, PCL and polysaccharides among many other blends (Avella et al., 2000; Imre & Pukánszky, 2013). Despite these approaches, the properties of the biopolymers in general are still not satisfactory and find difficulties in industrial applications (Rhim et al., 2013).
4. Materials and characterization techniques
et al. 2013) and in packaging industry as a substitute to traditional non-biodegradable plastics (Chandra and Rustgi 1998; Bittmann et al. 2013; Farmahini-Farahani et al. 2015; Pawar et al. 2015).
Figure 1.5 Schematic representation of the chemical structure of PHBV
Table 1.4 Melting temperatures and degree of crystallinity of PHB and different types of PHBV.
% of HV Tm1 Degree of crystallinity2 (%)
0 172.4 66
5 163.2 30
8 156.5 22
12 157.1 17
1 Melting temperature determined by step-scan differential scanning
2 Determined by wide angle X-ray diffraction (WAXRD)
The PHBV copolymer has improved mechanical properties over the PHB homopolymers. By increasing the HV content, the polymer become less brittle and more flexible with decreasing the elasticity modulus and increase in the elongation % (Avella et al., 2000). The decreased in the melting point help in avoiding degradation while processing.
biocompatible natural polymer. Starch is being widely used in food industries, paper making and as excipient in the pharmaceutical industry (Chiu & Solarek, 2009; Mason, 2009). In addition, starch is gaining an increasing attention in the packaging industry for its potential applications in the fields of food packaging, edible films and composting bags (J. Castaño et al., 2014; J. Castaño, Bouza, Rodríguez-Llamazares, Carrasco, & Vinicius, 2012). Starches from different botanical sources have different ratios and molecular weights of amylose and amylopectin and different crystalline structures that lead to different physical properties and thus different processability and possible applications (Johanna Castaño et al., 2017; Kim, Park, & Lim, 2015; Srichuwong, Sunarti, Mishima, Isono, & Hisamatsu, 2005; Young, 1984).
At molecular level, starch is mainly a polymer of glucose units that are connected together forming two macromolecules: amylose which is a helical α-(1–4) –linked D-glucose units [Figure 1.6], and amylopectin which is a highly-branched macromolecule of
Figure 1.6 Schematic representation of amylose.
Figure 1.8 Skeletal formula of quercetin.
4.2. Characterization techniques
4.2.1. Scanning electron microscopy (SEM)
Scanning electron microscopy (SEM) is an electron microscope where the electron beam is produced by an electron gun and accelerated using voltage from 1 to 30 kV. The electrons interact with the surface atoms of the scanned materials and the detector collects the signals of the secondary electrons emitted by the surface atoms excited by the electron beam [Figure 1.9]. Other types of signals like backscattered electrons or X-rays can be detected too (Kelsall, Hamley, & Geoghegan, 2015).
Figure 1.9 Diagram of FESEM.
being scanned by SEM. The technique used for this coating is a physical vapour deposition technique (PVD) called sputter coating. In this technique, a metal surface (target) is positioned as cathode and is eroded when bombarded with heavy fast inert gas ions (usually Ar) in conditions of gaseous glow discharge between an anode and cathode. As a result, the metal sputtered atoms will be deposited as a very thin even layer (few nanometres) on the surface of the sample. The sputter coating prevents the charging of the sample with the electron beam, improves the secondary electron emission, i.e. increases the signal to noise ratio, reduces the beam penetration and provide a protection for the beam sensitive materials.
4.2.2. Dynamic light scattering (DLS)
illuminated with a laser beam of a determined wavelength and the fluctuation of the light scattered is detected by a fast photon detector placed at a known angle. The laser used for DLS is normally of 632.8 nm or 532 nm. The continuous Brownian motion of the particles makes the scattering intensities to fluctuate continuously. Particles with different sizes have different Brownian motion speed, i.e. different translational diffusion coefficient (D). In case of small particles, the fluctuations of the scattered light are fast but of low amplitude and for large molecules vice versa (Braun, Cherdron, Rehahn, Ritter, & Voit, 2005). The DLS is measuring what called the hydrodynamic diameter of the particles dh, which is the diameter of the particles as well as the surrounding molecules of the solvent shell. The hydrodynamic diameter (dh) is determined using the Stokes-Einstein Equation (1.1):
𝑑" = '()*%& (1.1)
4.2.3. Static light scattering (SLS)
Unlike the DLS, the SLS technique depends on the measurement of the light scattering intensity at one or more angles. A laser beam is used for the illumination of the sample and usually several detectors are collecting the scattered light at different angles. This technique is useful for the determination of the weight-average molecular weight of polymers and for measuring the particle size in the range from tens of nanometres to few millimetres. The amount and the concentration required for performing the measurements are much higher in comparison with DLS.
4.2.4. Thermogravimetric analysis (TGA)
The furnace must be controlled through a software to insure the required rate for increasing the temperature. The thermal analysis can be done in an environment of different gases like N2, O2, air, argon and others. The weight of the sample (or the percentage of the initial sample weight) is plotted against the temperature making the TGA curves. The first derivation of the TGA curves is used for more in-depth understanding and analysis. The TGA is useful for the determination of decomposition temperature and the weight changes during the decomposition reaction. It is also used for tracking volatile rates of liquid mixtures or the percentage of water in some hydrophilic polymers.
4.2.5. Differential scanning calorimetry (DSC)
4.2.6. X-ray diffraction (XRD)
X-ray diffraction (XRD) is the diffraction of X-rays by a crystal that is the bases of X-ray crystallography.
X-ray crystallography is the use of X-ray diffraction to determine the structure of crystals or molecules. The technique involves directing a beam of X-rays at a crystalline sample and recording the diffracted X-rays on a photographic plate. The diffraction pattern consists of a pattern of spots on the plate, and the crystal structure can be worked out from the positions and intensities of the diffraction spots. X-rays are diffracted by the electrons in the molecules and if molecular crystals of a compound are used, the electron density distribution in the molecule can be determined (Daintith, 2008).
The two British scientists William Henry Bragg and his son William Lawrence Bragg have shared Nobel Prize of physics in 1915 for developing Bragg’s law [Equation 1.2] that explains relationship between the scattering pattern and the crystalline structure.
Where n is a positive integer, λ is the wavelength of the incident beam, d is the inter-planar distance and θ is the scattering angle [Figure 1.10].
Figure 1.10 Diagram of bragg's diffraction.
4.2.7. Ultraviolet–visible spectroscopy (UV–vis)
the intensity of the light beam after passing through the sample and compares it with the intensity of the light passing through the reference. The absorbance (A) is calculated through the software based on Beer-Lambert Law Equation (1.3):
A = log67
6 = 𝜀𝑙𝑐 (1.3)
4.2.8. Water vapour transmission rate (WVTR)
The steady-state transport properties of water vapour in barrier polymers are characterized by water vapour transmission rate (WVTR) (Dhoot et al., 2002). This parameter is critical for many industries especially for packaging of food and medications. Many equipment are available for performing this measurement.
Figure 1.11 Diagram of a WVTR testing cell.
4.2.9. Oxygen transmission rate (OTR)
the carrier gas and then calculated (Dhoot et al., 2002) [Figure 1.12]. OTR can be presented as volume of the oxygen gas transmitted through the film divided by the area and the time (cm3/m2.day).
The DSC, TGA, UV-vis, WVTR and OTR measurements of this thesis were performed in our laboratory (the laboratory of polymers, Escuela Universitaria Politécnica, Ferrol).
The DLS measurements were performed in the laboratory of Nanobiofar research group in the Centre for Research in Molecular Medicine and Chronic Diseases (CiMUS), University of Santiago de Compostela (USC) and in the laboratory of MatNaBio research group at the department of Physical-Chemistry II of the Faculty of Pharmacy of the Complutense University of Madrid (UCM).
All the FESEM micrographs were done in the Electronic and Confocal Microscopy unit of the (Rede de Infraestruturas de Apoio á Investigación e ao Desenvolvemento Tecnolóxico (RIAIDT)) of the University of Santiago de Compostela.
Objectives of the Thesis
The general objective of this thesis is the synthesis and characterization of nano and microparticles of biopolymers for food packaging applications.
For achieving this objective, we have developed four specific objectives as following:
1. Select an easy and appropriate technique for obtaining the desired nano and microparticles from both biopolymers: PHBV and starches from different botanical sources.
2. Characterization of the obtained nano and microparticles of both biopolymers.
3. Study the possibility of loading some of these nano and microparticles with natural antioxidants. Evaluate the loading percentage, antioxidant activity and the release kinetics.
Structure of the Thesis
The objectives of this thesis were developed as a part of the scientific project “Development of new materials based on polymeric bionanocomposites from natural resources [NanoCompBioPol]” funded by the Spanish Ministry of Economy and Finance. The thesis presents the part of the project that corresponds to the development of nano and microparticles from biopolymers and provides some possible applications for this particles in the food packaging area. The details of the thesis are presented in five main chapters preceded by an introduction chapter and followed by a general conclusions chapter as following:
Chapter 1. Introduction
It also introduces the main materials and characterization techniques used in this thesis.
Chapter 2. Preparation and characterization of nano and microparticles of poly(3-hydroxybutyrate-co-3-hydroxyvalerate) (PHBV) via emulsification / solvent evaporation and nanoprecipitation techniques.
This chapter describes the preparation and the characterization of nano and microparticles of poly(3-hydroxybutyrate-co-3-hydroxyvalerate) via two different preparation techniques: emulsification/solvent evaporation and nanoprecipitation and studies the effect of various conditions of preparation on the size and the morphology of the produced particles.
Chapter 3. Preparation of starch nanoparticles loaded with quercetin using nanoprecipitation technique.
starch origin on the quercetin loading percentage, the
release kinetics and the antioxidant activity of the produced
Chapter 4. Preparation of donut-shaped starch microparticles by aqueous-alcoholic treatment
This chapter reports a simple technique for the preparation of donut-shaped starch microparticles by thermal aqueous-alcoholic treatment.
Chapter 5. Starch edible films loaded with donut-shaped starch microparticles.
This chapter describes the preparation of thermoplastic starch edible films (TPS) loaded with donut-shaped starch microparticles from two different botanical origins. The chapter also discusses the improvement of the thermal and barrier properties of the starch films due to the incorporation of the donut-shaped starch microparticles.
Starch edible films loaded with donut-shaped starch-quercetin microparticles were prepared from two different botanical origins (pea and corn). The quercetin loading percentage and therefore the antioxidant activity for the microparticles was studied. The quercetin release kinetics through the starch films was studied in addition to the thermal stability of the films.
Chapter 7. General conclusions.
This chapter resumes the conclusions of each individual chapter and presents some general conclusions.
Each of the five main chapters was written in an independent way for its posterior planned publication. Each of these chapters is divided in an introduction, materials and methods section, results and discussion section and conclusions section. The references were presented separately for the introduction and for each individual chapter.
Ahmad, F. B., Williams, P. A., Doublier, J. L., Durand, S., & Buleon, A. (1999). Physico-chemical characterisation of sago starch. Carbohydrate Polymers, 38(4), 361–370.
Andrady, A. L. (2015). Plastics and Environmental Sustainability. Plastics and Environmental Sustainability.
Avella, M., Martuscelli, E., & Raimo, M. (2000). Review Properties of blends and composites based on poly(3-hydroxy)butyrate (PHB) and poly(3-hydroxybutyrate-hydroxyvalerate) (PHBV) copolymers. Journal of Materials
Science, 35(3), 523–545. http://doi.org/10.1023/A:1004740522751 Bodaghi, H., Mostofi, Y., Oromiehie, A., Ghanbarzadeh, B., & Hagh, Z. G. (2015). Synthesis of clay-TiO2 nanocomposite thin films with barrier and photocatalytic properties for food packaging application. Journal of Applied Polymer Science, 132(14), 4–11. http://doi.org/10.1002/app.41764
Bose, S., Du, Y., Takhistov, P., & Michniak-Kohn, B. (2013). Formulation optimization and topical delivery of quercetin from solid lipid based nanosystems. International Journal of
Pharmaceutics, 441(1–2), 56–66.
Braun, D., Cherdron, H., Rehahn, M., Ritter, H., & Voit, B. (2005). Polymer Synthesis : Theory and Practice. New York.
Brockgreitens, J., & Abbas, A. (2016). Responsive Food Packaging: Recent Progress and Technological Prospects.
Comprehensive Reviews in Food Science and Food Safety, 15(1), 3–15. http://doi.org/10.1111/1541-4337.12174
Polymer Letters, 8(11), 791–808.
Castaño, J., Bouza, R., Rodríguez-Llamazares, S., Carrasco, C., & Vinicius, R. V. B. (2012). Processing and characterization of starch-based materials from pehuen seeds (Araucaria araucana (Mol) K. Koch). Carbohydrate Polymers, 88(1), 299–307. http://doi.org/10.1016/j.carbpol.2011.12.008
Castaño, J., Rodríguez-Llamazares, S., Contreras, K., Carrasco, C., Pozo, C., Bouza, R., … Giraldo, D. (2014). Horse chestnut
(Aesculus hippocastanum L.) starch: Basic physico-chemical characteristics and use as thermoplastic material. Carbohydrate Polymers, 112, 677–685.
Castaño, J., Rodríguez-Llamazares, S., Sepúlveda, E., Giraldo, D., Bouza, R., & Pozo, C. (2017). Morphological and structural changes of starch during processing by melt blending. Starch - Stärke, 68, 1–9. http://doi.org/10.1002/star.201600247
Castro-Aguirre, E., Iñiguez-Franco, F., Samsudin, H., Fang, X., & Auras, R. (2016). Poly(lactic acid)—Mass production, processing, industrial applications, and end of life. Advanced Drug Delivery Reviews, 107, 333–366. http://doi.org/10.1016/j.addr.2016.03.010 Chandra, R., & Rustgi, R. (1998). Biodegradable polymers. Progress in Polymer Science, 23(7), 1273–1335.
Chartoff, R. P., Sircar, A. K., Chartoff, R. P., & Sircar, A. K. (2004). Thermal Analysis of Polymers. In Encyclopedia of
Polymer Science and Technology. Hoboken, NJ, USA: John Wiley & Sons, Inc. http://doi.org/10.1002/0471440264.pst367
Chiu, C. wai, & Solarek, D. (2009). Modification of Starches. Starch (Third Edit). Elsevier Inc. http://doi.org/10.1016/B978-0-12-746275-2.00017-3
Dechene, E. B. (1951). The relative stability of rutin and quercetin in alkaline solution. Journal of the American Pharmaceutical Association., 40(10), 495–497.
Dhoot, S. N., Freeman, B. D., Stewart, M. E., Dhoot, S. N., Freeman, B. D., & Stewart, M. E. (2002). Barrier Polymers. In Encyclopedia of Polymer Science and Technology. Hoboken, NJ, USA: John Wiley & Sons, Inc.
Encyclopædia Britannica. (2017). Plastic. In Encyclopædia Britannica. Encyclopædia Britannica, inc. Retrieved from https://www.britannica.com/science/plastic
Esmailzadeh, H., Sangpour, P., Shahraz, F., Hejazi, J., & Khaksar, R. (2016). Effect of nanocomposite packaging containing ZnO on growth of Bacillus subtilis and Enterobacter aerogenes. Materials Science and Engineering C, 58, 1058–1063.
European bioplastics. (2016). Bioplastic market data. European Bioplastics, 4. Retrieved from
European bioplastics. (2017a). Bioplastics: facts and figures. European Bioplastics, 26. Retrieved from http://docs.european-bioplastics.org/publications/EUBP_Facts_and_figures.pdf European bioplastics. (2017b). Frequently asked questions on bioplastics. European Bioplastics, 26. Retrieved from
http://docs.european-bioplastics.org/publications/EUBP_FAQ_on_bioplastics.pdf Geyer, R., Jambeck, J. R., & Law, K. L. (2017). Production, use, and fate of all plastics ever made. Science Advances, 3(7), e1700782. http://doi.org/10.1126/sciadv.1700782
mice by anti-inflammatory and antioxidant mechanisms. Journal of Natural Products, 76(2), 200–208.
Gunaratne, L. M. W. K., & Shanks, R. A. (2005). Multiple melting behaviour of poly(3-hydroxybutyrate-co-hydroxyvalerate) using step-scan DSC. European Polymer Journal, 41, 2980–2988. http://doi.org/10.1016/j.eurpolymj.2005.06.015
He, X., & Hwang, H. M. (2016). Nanotechnology in food science: Functionality, applicability, and safety assessment. Journal of Food and Drug Analysis, 24(4), 671–681.
Imre, B., & Pukánszky, B. (2013). Compatibilization in bio-based and biodegradable polymer blends. European Polymer Journal, 49(6), 1215–1233. http://doi.org/10.1016/j.eurpolymj.2013.01.019 Javadi, A., Pilla, S., Gong, S., & Turng, L.-S. (2011). Biobased and Biodegradable PHBV-Based Polymer Blends and Biocomposites : Properties and Applications. In Handbook of Bioplastics and Biocomposites Engineering Applications (pp. 372–396). Hoboken, NJ, USA: John Wiley & Sons, Inc.
Jeszka-Skowron, M., Krawczyk, M., & Zgoła-Grześkowiak, A. (2015). Determination of antioxidant activity, rutin, quercetin, phenolic acids and trace elements in tea infusions: Influence of citric acid addition on extraction of metals. Journal of Food Composition and Analysis, 40, 70–77.
Joye, I. J., & McClements, D. J. (2014). Biopolymer-based
nanoparticles and microparticles: Fabrication, characterization, and application. Current Opinion in Colloid & Interface Science, 19(5), 417–427. http://doi.org/10.1016/j.cocis.2014.07.002
Chemical Physics, 16(25), 12802–12811. http://doi.org/10.1039/c4cp00864b
Kelsall, R. W., Hamley, I. W., & Geoghegan, M. (Eds.). (2015). Nanoscale Science and Technology. Wiley.
Kim, H. Y., Park, S. S., & Lim, S. T. (2015). Preparation, characterization and utilization of starch nanoparticles. Colloids and Surfaces B: Biointerfaces, 126, 607–620.
Kumar, N., Ezra, A., Ehrenfroind, T., Krasko, M. Y., Domb, A. J., Kumar, N., … Domb, A. J. (2003). Biodegradable polymers, medical applications. In Encyclopedia of Polymer Science and Technology. Hoboken, NJ, USA: John Wiley & Sons, Inc. http://doi.org/10.1002/0471440264.pst027
Laycock, B., Halley, P., Pratt, S., Werker, A., & Lant, P. (2014). The chemomechanical properties of microbial
polyhydroxyalkanoates. Progress in Polymer Science, 39(2), 397– 442. http://doi.org/10.1016/j.progpolymsci.2013.06.008
Li, H., Zhao, X., Ma, Y., Zhai, G., Li, L., & Lou, H. (2009). Enhancement of gastrointestinal absorption of quercetin by solid lipid nanoparticles. Journal of Controlled Release, 133(3), 238– 244. http://doi.org/10.1016/j.jconrel.2008.10.002
Lightfoot Vidal, S., Rojas, C., Bouza Padin, R., Perez Rivera, M., Haensgen, A., Gonzalez, M., & Rodriguez-Llamazares, S. (2016). Synthesis and characterization of
polyhydroxybutyrate-co-hydroxyvalerate nanoparticles for encapsulation of quercetin. Journal of Bioactive and Compatible Polymers, 31(5), 439–452. http://doi.org/10.1177/0883911516635839
Malmir, S., Montero, B., Rico, M., Barral, L., & Bouza, R. (2017). Morphology, thermal and barrier properties of biodegradable films of poly (3-hydroxybutyrate-co-3-hydroxyvalerate) containing cellulose nanocrystals. Composites Part A: Applied Science and Manufacturing, 93, 41–48.
Mason, W. R. (2009). Starch Use in Foods. Starch (Third Edit). Elsevier Inc. http://doi.org/10.1016/B978-0-12-746275-2.00020-3 Mihindukulasuriya, S. D. F., & Lim, L. T. (2014). Nanotechnology development in food packaging: A review. Trends in Food Science and Technology, 40(2), 149–167.
Mohan, L., Anandan, C., & Rajendran, N. (2016). Drug release characteristics of quercetin-loaded TiO nanotubes coated with chitosan. International Journal of Biological Macromolecules, 4–9. http://doi.org/10.1016/j.ijbiomac.2016.04.034
Montero, B., Rico, M., Rodríguez-Llamazares, S., Barral, L., & Bouza, R. (2016). Effect of nanocellulose as a filler on
biodegradable thermoplastic starch films from tuber, cereal and legume. Carbohydrate Polymers.
Mousa, M. H., Dong, Y., & Davies, I. J. (2016). Recent advances in bionanocomposites: Preparation, properties, and applications. International Journal of Polymeric Materials and Polymeric Biomaterials, 65(5), 225–254.
Notta-Cuvier, D., Odent, J., Delille, R., Murariu, M., Lauro, F., Raquez, J. M., … Dubois, P. (2014). Tailoring polylactide (PLA) properties for automotive applications: Effect of addition of designed additives on main mechanical properties. Polymer Testing, 36, 1–9.
Oever, M. Van Den, Molenveld, K., Zee, M. Van Der, & Bos, H. (n.d.). Bio-based and biodegradable plastics – Facts and Figures. Oksman, K., Aitomäki, Y., Mathew, A. P., Siqueira, G., Zhou, Q., Butylina, S., … Hooshmand, S. (2016). Review of the recent developments in cellulose nanocomposite processing. Composites Part A: Applied Science and Manufacturing, 83, 2–18.
Pérez, S., Baldwin, P. M., & Gallant, D. J. (2009). Structural features of starch granules I. Starch (Third Edit). Elsevier Inc. http://doi.org/10.1016/B978-0-12-746275-2.00005-7
PlasticsEurope. (2016). Plastic - the Facts 2016, 38. Retrieved from http://www.plasticseurope.es/Document/plastics---the-facts-2016-15787.aspx?FolID=2
Rhim, J.-W., Park, H.-M., & Ha, C.-S. (2013). Bio-nanocomposites for food packaging applications. Progress in Polymer Science, 38(10–11), 1629–1652.
Rico, M., Rodríguez-Llamazares, S., Barral, L., Bouza, R., & Montero, B. (2016). Processing and characterization of polyols plasticized-starch reinforced with microcrystalline cellulose. Carbohydrate Polymers, 149, 83–93.
Srichuwong, S., Sunarti, T. C., Mishima, T., Isono, N., &
Hisamatsu, M. (2005). Starches from different botanical sources I: Contribution of amylopectin fine structure to thermal properties and enzyme digestibility. Carbohydrate Polymers, 60(4), 529–538. http://doi.org/10.1016/j.carbpol.2005.03.004
Stevens, E. S. (2003). Environmentally Degradable Plastics. In Encyclopedia of Polymer Science and Technology. Hoboken, NJ, USA: John Wiley & Sons, Inc.
van Soest, J. J. G., Hulleman, S. H. D., de Wit, D., & Vliegenthart, J. F. G. (1996). Crystallinity in starch bioplastics. Industrial Crops and Products, 5(1), 11–22.
Wang, G., Wang, J. J., Chen, X. L., Du, L., & Li, F. (2016).
Quercetin-loaded freeze-dried nanomicelles: Improving absorption and anti-glioma efficiency in vitro and in vivo. Journal of
Controlled Release, 235, 276–290.
Young, A. H. (1984). Chapter VIII – Fractionation of starch. In Starch: Chemistry and Technology (Second edi, pp. 249–283). http://doi.org/10.1016/B978-0-12-746270-7.50014-8
Yu, H., Yan, C., & Yao, J. (2014). Fully biodegradable food packaging materials based on functionalized cellulose nanocrystals/poly(3-hydroxybutyrate-co-3-hydroxyvalerate) nanocomposites. RSC Adv., 4(104), 59792–59802.
2. Preparation and characterization of nano and
poly(3-hydroxybutyrate-co-3-hydroxyvalerate) (PHBV) via emulsification /
solvent evaporation and nanoprecipitation
Polymeric nano and microparticles have many applications in different areas such as drug delivery systems, biosensors, analytical and catalysis agents, tissue engineering and for environmental applications (Joye & McClements, 2014; Lassalle & Ferreira, 2007; Retama, Mecerreyes, Ruiz, & Lopez-Cabarcos, 2005; Rico et al., 2016). Many methods are being followed to prepare polymeric particles from a lot of polymers based on both chemical and physical behaviour of the polymers and their monomers (Rao & Geckeler, 2011; Vauthier & Bouchemal, 2009). Studying the factors that affect the morphological, chemical and physical properties of the produced particles is a key step for controlling the production of the particles and addressing their appropriate applications.
containing a surfactant. The formation of the stable emulsion is followed by evaporation of the polymer solvent which is usually a volatile organic solvent. The emulsion is made by simple magnetic or mechanical stirring. The stirring could be followed by a further step of sonication (Musyanovych, Schmitz-Wienke, Mailänder, Walther, & Landfester, 2008). The emulsification can be performed also by ultrasonication using a high-power ultrasound (Iqbal, Valour, Fessi, & Elaissari, 2015; Lu et al., 2012). The incorporated surfactant stabilizes the emulsion, while its concentration affects the size of the droplet of the emulsion. The evaporation of the solvent is carried out by mild heating for several hours or under low pressure leaving behind polymeric nano and microparticles suspended in the aqueous phase (Lionzo, Ré, Guterres, & Pohlmann, 2007).
solvents and saline solutions can also be used (Galindo-Rodriguez, Alle, Fessi, & Doelker, 2004; Schubert et al., 2011). The precipitation of the particles of the polymer occurs when they are exposed to the anti-solvent by slow addition of one phase in the other while sonication or stirring or both. Nanoprecipitation does not require the use of surfactants. However, they could be added to the anti-solvent to stabilize the nanoparticles in some cases (Bilati, Allémann, & Doelker, 2005). The polymer nature, polymer solvent and polymer concentration, solvent/non solvent ratio, interactions and the way of addition are very important for the success of nanoprecipitation process and to get the desired size and morphology of the particles (Legrand et al., 2007).
type, surfactant concentration and polymer concentration on the size and the morphology of the produced nano and microparticles of PHBV via the traditional emulsification/solvent evaporation method (Bouza et al., 2016; Q. Chen et al., 2016; W. Li et al., 2014; Lightfoot Vidal et al., 2016; Pacheco, Amaral, Reis, Marques, & Correlo, 2015; Pich, Schiemenz, Corten, & Adler, 2006; Pramual et al., 2016).
The morphology and the size of the nano and microparticles of PHBV produced via both techniques were analysed using field emission scanning electron microscope (FESEM), static mode light scattering (SLS) and dynamic light scattering (DLS).
2. Materials and methods 2.1. Materials and reagents
Poly(3-hydroxybutyrate-co-3-hydroxyvalerate) with 12% hydroxyvalerate (HV) content (PHBV) Mw: 240,000, was supplied by Goodfellow Cambridge limited, UK. Sodium dodecyl sulphate (SDS), chloroform, dichloromethane, ethanol, methanol and dimethylformamide (DMF) were purchased from Scharlau, Spain. Polyvinyl alcohol (PVA) 86.7-88.7 mol% hydrolysis Mw: 31,000 (Mowiol® 4-88) and sodium chloride were purchased from Sigma Aldrich, Germany. All chemicals were used without further purification. The water used in both techniques and washing was purified on a Milli-Q ultrapure system (Millipore, Molsheim, France).
2.2. Preparation of the particles via emulsification/solvent
Table 2.5 Preparation conditions of PHBV particles via emulsification/solvent evaporation.
No PHBV concentration
% w/v Surfactant
left overnight at 40 ºC with stirring for evaporating the dichloromethane. A second series of preparations was performed repeating the same previously mentioned procedure but with 0.1% PHBV in dichloromethane (samples 7ES-10ES).
The same procedure was repeated using different concentrations of PVA as surfactant [Table 2.5, samples 12ES-17ES]. In this case 100 mL of organic phase were added to 300 mL of aqueous phase, the stirring was performed with mechanical stirrer as the magnetic stirring is not adequate for the viscous PVA solution. Variation of the PVA concentration and the polymer concentration were performed to study the effect of those factors on the morphology and the size of the produced particles.
2.3. Preparation of the particles via nanoprecipitation
ultrasonication or mechanical stirring at room temperature. The organic solvent was evaporated and the particles were washed several times with water, or washed directly without evaporation in case of using DMF as the boiling point of DMF is higher than water. The collected particles were lyophilized to be characterized.
the different procedures followed for the preparation of PHBV particles via nanoprecipitation.
Table 2.6 Preparation conditions of PHBV particles via nanoprecipitation.
The morphology of the particles was characterized using a Carl Zeiss ultra plus field emission scanning electron microscope (FESEM) operated at 3 kV (Carl Zeiss, Germany). The particles were previously sputter-coated with iridium using QUORUM Q150T-S turbo-pumped sputter coater (Quorum Technologies Ltd, UK).
The size of the particles was determined using static mode light scattering (SLS) Saturn DigiSizer II 5205 (Micromeritics Instrument Corporation, U.S.A) and dynamic light scattering (DLS) Zetasizer 3000 (Malvern Instruments, UK). The size of the particles was measured while dispersed in deionized water.
3. Results and discussion.
3.1. Emulsification/solvent evaporation
ultrasonication were performed in each group. The produced particles were collected and analysed to study the effect of those factors on their size and morphology.
3.1.1. Emulsification using SDS
Figure 2.13 Micrograph of a microparticle of PHBV prepared by emulsification/solvent evaporation method using 1% PHBV in dichloromethane and SDS as surfactant in a concentration of 1% (2ES).
those nanoparticles were always accompanied with relatively wide size range of microparticles except when very high SDS concentrations were used. The nanoparticles can be easily separated from the microparticles by filtration and ultra-filtration.
Figure 2.15 shows the changes in the morphology and in the particle size distribution by changing the SDS concentration.
Figure 2.14 Static light scattering plot. Particle diameter in µm vs incremental volume percent for different PHBV samples prepared by emulsification/solvent evaporation using different concentrations of SDS as
Figure 2.15 Micrograph of nano and microparticles of PHBV prepared by emulsification/solvent evaporation method using 1% PHBV in dichloromethane and SDS as surfactant with concentrations: 0.3% (a: 1ES),
1% (b: 2ES), 2% (c: 3ES), 5% (d: 4ES), 10% (e: 5ES), 15% (f: 6ES).
Figure 2.16 Micrograph of nano and microparticles of PHBV prepared by emulsification/solvent evaporation method using SDS as surfactant with concentrations: 1% PHBV, 1% SDS (a: 2ES), 0.1% PHBV 1% SDS (b: 7ES),
1% PHBV 2% SDS (c: 3ES), 0.1% PHBV 2% SDS (d: 8ES), 1% PHBV 5% SDS (e: 4ES), 0.1% PHBV 5% SDS (f: 9ES), 1% PHBV 10% SDS (g: 5ES),
It seems that increasing the concentration of the surfactant has no significant effect on the size at a very low polymer concentration (0.1%) until reaching very high SDS concentration (10%). The produced particles in those series of preparation were microparticles between 2-10 µm with a population of nanoparticles of around 380 nm. When using a concentration of 10% SDS, the microparticles were between 1-2 µm while maintaining the same population of nanoparticles [Figure 2.17].
Figure 2.17 Static light scattering plot. Particle diameter in µm vs incremental volume percent for different PHBV samples prepared by emulsification/solvent evaporation using different concentrations of SDS as
3.1.2. Emulsification using PVA
Figure 2.18 Static light scattering plot. Particle diameter in µm vs incremental volume percent for different PHBV samples prepared by emulsification/solvent evaporation using different concentrations of PVA as
surfactant and polymer concentration of 1%.
The analysis of the particles produced by various polymer concentrations shows that by decreasing the PHBV concentration to 0.5% while maintaining the PVA concentration at 10%, the particle size distribution decreased slightly. Most of particles were around 1-2 µm. Lowering the concentration of PHBV to 0.1% produced nanoparticles of around 380 nm in addition to microparticles of 1-2
Figure 2.20 Static mode light scattering plot. Particle diameter in µm vs incremental volume percent for different PHBV samples prepared by emulsification/solvent evaporation using solution of 10% PVA as surfactant
and three different polymer concentrations.
using SDS were smoother than those produced by PVA at the same surfactant concentration.
For establishing a comparison between the effect of both utilized surfactants, it can be said that at high concentration of surfactant (10%), PVA produces more homogenous and smaller microparticles. However, nanoparticles were obtained besides the microparticles when using SDS in the same concentration. More percentage of nanoparticles can be produced by increasing the SDS concentration and/or decreasing the polymer concentration. Obtaining only nanoparticles could be achieved simply by filtration the produced mixture of nano and microparticles. At low surfactant concentration (5%), the particles produced using SDS were smaller and the particle size distribution was narrower.
SDS, while with PVA the mean size was 297 ± 93 nm. The size distribution was significantly wider utilizing PVA [Figure 2.21]. Göz et al. (Göz & Karakeçili, 2016) and Lightfoot Vidal et al. (Lightfoot Vidal et al., 2016) have reported the use of the high-speed homogenizer for the preparation of nanoparticles of PHBV. The mean particle size of the nanoparticles obtained by Lightfoot Vidal et al. was around 611nm before filtration and 234 nm after filtration. The surfactant used was PVA 85,000–124,000 molecular weight in a concentration of 0.025%.
Figure 2.21 Dynamic light scattering plot showing the size distribution of two PHBV samples prepared by emulsification/solvent evaporation of 1% PHBV in dichloromethane using two different surfactants, SDS (11ES) and
Although the nanoprecipitation technique is one of the simplest way for the preparation of the nanoparticles, it is necessary to adjust many parameters to get the desired particles with proper size distribution and morphology and to evade any possible aggregation. The polymer concentration should be relatively low. The ratios between solvent / nonsolvent and nonsolvent / co-nonsolvent (if any) must be in the acceptable range. The addition process and the stirring or sonication rate and power have considerable impact on the whole process (Schubert et al., 2011).
3.2.1. Ethanol as anti-solvent
dissolve the particles (Poletto et al., 2008). The addition was accompanied with mechanical stirring at 300 rpm.
Figure 2.22 Micrograph of nano and microparticles of PHBV prepared by nanoprecipitation method using 1% PHBV in dichloromethane and a mixture of ethanol and water as anti-solvent: 100% ethanol (a: 1NE), 80%
ethanol/20% water (b: 7NE), 70% ethanol/30% water (c: 8NE), 70% ethanol/30% water applying ultrasonication (d: 9NE).
anti-solvent has no significant effect on the size or the morphology of the nanostructures.
The polarity of the ethanol was increased by the addition of water (Wyman, 1931). The water / ethanol ratio should not exceed 3:7. A solution of ethanol with more than 30% of water is not miscible with dichloromethane and will make an emulsion upon stirring instead of the desired diffusion.
Figure 2.23 Dynamic light scattering plot showing the size distribution of PHBV nanoparticles prepared by nanoprecipitation of 1% PHBV in dichloromethane using 70% ethanol/30% water applying ultrasonication